EFFICIENT DETERMINATION OF MECHANICAL PROPERTIES OF CARBON FIBREREINFORCED LAMINATED COMPOSITE PANELS


 Sharlene Morgan
 7 months ago
 Views:
Transcription
1 EFFICIENT DETERMINATION OF MECHANICAL PROPERTIES OF CARBON FIBREREINFORCED LAMINATED COMPOSITE PANELS Umar Farooq and Peter Myler Faculty of Engineering and Advanced Sciences, University of Bolton BL3 5AB, United Kingdom ABSTRACT This paper is concerned with integrating experimental and theoretical methods supported by numerical simulations to efficiently determine mechanical properties of carbon fibrereinforced laminated composite panels. Ignition loss experiments were conducted for eight, sixteen, and twentyfour ply laminates to approximate fibre volume fractions by weights. Rule of mixture was utilised to approximate basic mechanical properties (Young s and shear moduli and Poisson s ratios) for a lamina. The mechanical properties were utilised to develop coefficients of stiffness and compliance matrices. The coefficient matrices are used in constitutive equations to align offaxis fibres and applied load to midplane direction in twodimensional formulations. Based on the twodimensional formulations stacking sequences of threedimensional laminate layupswere developed without resorting to threedimensional micromacro mechanics. The formulations laminates were then coded in commercial software MATLAB TM to predict mechanical properties. Tensile and flexural physical tests of the laminates were also conducted to validate the simulation obtained mechanical properties. Comparisons of mechanical properties have shown good agreement (over 90%) between laminates having different types of stacking sequences. Based on comparison of the results an efficient and systematic twodimensional methodology is proposed to predict mechanical properties of threedimensional laminates. Keywords: A. composite laminates, B. mechanical properties, C. tensile test, D. bending test. 1. INTRODUCTION The fibrereinforced composite laminates are being increasingly used in structural design as a building block of modern commercial aircrafts parts due to their high specific strength, high specific stiffness, light weight, and superior inplane properties [1] and [2]. When a material is characterised experimentally, engineering constants are measured instead of the stiffness or the compliance. This is because engineering constants can be easily defined and interpreted in terms of simple state of stress and strain used in design development and analysis. Mechanical properties of the test standard laminates are obtained from static testing before using them as a structural component. But laminates are anisotropic in nature and have to undergo series of experiments to obtain their properties. Moreover, parts have certain characteristics of shape, rigidity, and strengthhence their testing could be complicated [3]. Knowledge of mechanical properties to evaluate their performance and identify load bearing parameters that influence strength and response of laminates (fibre, matrix and interfaces) require efficient techniques [4]. In the literature common existing experimental methods consist of: tensile, compression, flexural, shear modulus, Iosipescu, and v notchrail prevail. Most of the methods are detailed in (ASTM: D7264). A large number of factors affect property determination of laminates such as: dispersion and distribution of matrix and filler, compatibility, nature, and material processing technology [5] and [6].Hence series of tests are conducted for screening the properties before their integration in full scale structures or putting them into work. At the same time, physical testing of laminates is very inconvenient and resource consuming. Interfacial structural element and morphology also affect quality of the evaluated mechanical properties [7] and [8]. Thus larger spantodepth ratios are used to reduce the adverse influence of the interfaces [9] and [10]. Many experimental test methods use different geometries and holdingfixtures for laminates that produce different data. Influence of shear effects in the displacements is another important factor [11] and [12]. The laminates subjected to offaxis loading system present tensileshear interactions in its plies. The tensileshear interactions lead to distortions and local microstructural damage and failure, so in order to obtain equal stiffness in all offaxis loading systems, a composite laminate have to be balanced angle plies [13]. Some of the studies complement physical testing by using Rule of Mixture (ROM). The method could be useful approximate laminates with aligned reinforcement (stiff along the fibres) and very weak (transverse to the fibres direction). Furthermore, the ROM method relates material properties of the laminates into algebraic set of equations that are easier to code and solve using computer [14]. Still use of the method is limited for cases of tensileshear interaction if the offaxis loading system does not coincide with the main axes of a single lamina or if the laminate is not balanced [15]. The solution to obtain equal stiffness of laminates subjected in all directions within a plane is presented by various authors by stacking and bonding together plies with different fibres orientations [16] and [17]. The allocation of the appropriate input engineering parameters such as the effective elastic moduli and the associated Poisson s Ratios for the materials based on the theory of linear elasticity and their limitations are described in [18]. Theoretical approach to compute the elastic constants of laminates based on epoxy resin reinforced alternatively with glass, HM carbon, HS carbon and Kevlar49 fibres are reported in [19] and [20]. The laminates taken into account the plies sequence [0/45/90/45/0] in order to obtain equal 1375
2 stiffness in all loading systemssubjected to offaxis loading systems. The elastic constants were also determined for laminates have to present balanced angle plies [21]. Review of the literature revealed that most of the existing studies are experimental where many test methods have limitations with testing and data logging systems. Majority of the analytical studies are based on ROM methods and limited to simplified twodimensional formulation. In the present study, effective mechanical properties for threedimensional laminates were approximated utilising twodimensional laminated plate theory. Quantities of volume fractions by weight were determined with ignition loss method. The volume fractions were utilised in ROM relations to approximate basic mechanical properties. The mechanical properties were utilised in laminated plate formulation to include loaddeformation influence. The formulation was then coded in MATLAB TM to approximate the mechanical properties. Tensile and flexural tests were also conducted to compare and validate the results. Comparisons of experimental and simulation results were found within acceptable agreement. The study demonstrated that twodimensional laminated plate formulation can be systematically and effectively utilised to evaluate a range of engineering constants of threedimensional laminates. 2. MATERIAL AND METHODS 2.1 Geometric properties of the laminates Composites are heterogeneous materials hence full characterisation of their properties is difficult as various processing factors can influence the properties such as misaligned fibres, fibre damage, nonuniform curing, cracks, voids and residual stresses. These factors are assumed to be negligible when care is taken in the manufacturing process. It is for this reason that the purpose specific aerospace specialist fabricated laminates (manufacturers supplied) were used here. For a better understanding of the laminate, a brief illustration of the coordinate systems used is shown in Figure1. The XYZ system is the global coordinates system. The system is the local material coordinates system defined foreach ply with the 1 axis representing the fibre direction, the 2 axis representing the direction perpendicular to the fibre direction and the 3 axis representing the outofplane direction. A typical 8Ply laminate is shown in Figure2. Figure1. Coordinate systems convention. a) Fibre angle b) Satinweave property Figure2. Schematic of 8Ply symmetric laminate. The laminates are also assumed to be void free, linear elastic with plane dimensions 150mm x 120mm with fibre horns technique of every fourth layer. Average thicknesses of the laminates consisting of eight, sixteen, and twentyfour plies with layup sequence are given in Table
3 Laminates Table1. Measured thickness of laminates. Code: Fibredux 914C No. of ply Layup code Average thickness mm 8 [0/90/45/45] S [0/90/45/45] 2S [0/90/45/45] 3S 7.2 The material properties are given in Table2. Table2. Material properties of the laminates. Property parameters Tensile Modulus E xx, E yy in 0 0 & 90 0 and Units Fibredux 914C Gpa 230 in 45 0 & Gpa 23 Shear Modulus G 12 Gpa 88 Poisson s Ratio ( 12 ) Volume fractions obtained from ignition loss method Densities of fibres and resin matrix contents were determined experimentally by weighing them in air. The ignition loss method (ASTM: D ) was used for polymeric matrix composites containing fibres that do not lose weight at high temperature. In this method, cured resin is burnt off from a small test at C in a muffle furnace. After burning for three hours at C the density of fibres comes down to 1.8g/cm 3 and that of the matrix as 2.09g/cm 3. Three laminates were tested and fibre percentages (residue mass/sample mass) per unit volume (cm 3 ) were calculated as shown in Table3 given below. The density quantities shown in column 7 were then utilised in Rule of Mixture to calculate volume fraction of carbon fibresas shown in column 8 of the same Table. Table3. Fibre contents of laminates. Sample Heated up to C Sample Residue Density Length Width Depth mass g mass g g/cm 3 Carbon fibre % 8Ply Ply Ply METHODOLOGY TO DETERMINE MECHANICAL PROPERTIES Conventions used in this study: a) Elastic constants are expressed throughout in normal format rather than italic to keep uniformity with the other variables in equations. b) Micromechanics does not refer to mechanical behavior at the molecular level rather it looks at components of a composite (matrix and fibre) and tries to predict the behavior of the assumed homogeneous composite material. 3.1 Micromechanics methods A lamina (heterogeneous at the constituent level) forms the building block of laminated composites based structures. The mechanical and physical properties of the lamiae (reinforcement and matrix) and their interactions are examined on a microscopic level on various degrees of simplifications. Fibre and matrix densities are measured and converted into respective fibre volume fractions that form basis for approximation of engineering properties (see Figure3). c) The behavior of the lamina is called macromechanics. Most of the structural parts use laminates that consist of several plies with different orientations connected together through a bonding interface. 1377
4 ρ c V c = ρ f V f + ρ V (Rule of mixture for density) (6) Eq. (1) can be rearranged as V c = ( W f )+ W c W f ρ f ρm Wc ρc (7) Figure3. Micro and macromechanics processfor property determination. The measured densities and fibre volume fractions of a laminate can be related to its ingredients using Rule of Mixture and utilised to determine volume fractions by weight. The volume and weight fractions are given in Eq. (1) and Eq. (2) below: V c = V f + V + V = = composite volume (1) Where: V f = f =fibre volume fraction; V = c m = matrix volume fraction; and V = v = void volume c c fraction The weight fractions are given with the relation: W c = W f + W = composite weight (void weight is neglected) (2) Where: W f = f = fibre weight fraction and c W = m = matrix weight fraction c The density (ρ = ) is used to approximate volume fractions = density ρ c = c ρ c W f + W m ρ f ρm (3) = f + c f (4) ρ f ρ m Where: The symbols W, V, and ρ represent weight, volume, and density. The subscripts c, f, m, and v denote composite, fibre, matrix, and void, respectively. Fibre volume fraction from densities neglecting void contents zero is: FVF = ρ c ρ m ρ f ρ m fraction (8) The fibre volume fraction from fibre weight FVF = [ + ρ F ρ m ] (9) Where W = ρ F [ρ m +(ρ f ρ m ).V] (10) The cured ply thickness from ply weight ( CPT = F ρ f (11) Where: FVF = fibre volume fraction FWF = fibre weight fraction ρ c = density of composite (g/cm 3 ) ρ m = density of cured resin/hardener matrix (g/cm 3 ) ρ f = density of fibres (g/cm 3 ) W F = fibre area weight of each ply (g/m 2 ) CPT (mm) = Cured ply thickness calculated from volume fraction. = ( W f )+ W c W f ρ f ρm Wc ρc (5) From the Eq. (9) and Eq. (10) fibre volume fraction by weight was determined as 54% using MATLAB TM code Figure
5 % Computing values from mat lab % Effective Length = Length 120 mm Grips 30 mm = 90 mm l =90;b =23; delta =0.4; ply=input('enter no of ply'); if(ply==8)% p is applied load p =25; h =2.4; elseif (ply==16) p=190; h=4.8 else (ply==24) p=600;h = 7.2; end mom =p*l/2; i= 23*(h^3)/12; smax=(mom*(h/2))/i; elast=(p*l^3)/(48*delta*i; epsi=smax/elast; disp(mom);disp(i);disp(smax);disp(elast);disp(epsi) % Values computed from Matlab software for sample D % Average length l1= 12.84;l2=12.38;l=(l1+l2)/2; %Average width w1= 11.4;w2=11.54;w= (w1+w2)/2; %Average thickness t1= 6.84;t2=4.68;t=t1+t2; % Volume of sample D volume = l*w*t; disp('volume of the sample is'); disp(volume); % sample mass and density smass = ;denst1=smass/volume; disp('density of the sample is'); disp(denst1); % Residue mass and density residu = ; rmass = ; denst2 = rmass/volume; disp('density of the residue is ');disp(denst2) % Calculations for volume and weight fibre fractions imass = ; % initial mass fmass = ; % final mass ratio1 =fmass/imass; ratio1= 1/ratio1; ratio1=ratio11 % values found from the Internet rowf = 1.8; % fibre density rowm = 2.09; % matrix density ratio2=rowf/rowm; denom1 = ratio1*ratio2; denom1 = denom1+1; fvf = 1/denom1; disp (fvf)= % fibre weight fraction from fibre volume fraction rowf= 1.8;rowm=2.09;fvf = ; denom1 = rowm+(rowfrowm)*fvf;fwf=rowf*fvf/denom1; disp(fwf) = Figure4. MATLAB TM code to compute volume fractions by weight Mechanical properties of a lamina By the rule of mixtures, the modulus of a composite is defined as the combination of the modulus of the fibre and the modulus of the matrix that are related to the volume fractions of the constituent materials [11]: E c = E f V f + E V (12) Where: E c is the modulus of elasticity of the composite Assuming perfect bonding very small modulus of matrix, the equations for calculating ply moduli are written as: E = E f V f + E V (Longitudinal Young s modulus) (13) E = m f + f m m f (Transverse Young s modulus) (14) G = f m m f + f m (Inplane shear modulus) (15) ν = ν f V f + ν V (Poisson s ratios) (16) Determination of critical volume fractions Fibre volume fraction using Eq. (9) and Eq. (10) can be rewritten as: V f = f ρ f [ f ρ f + W f ρ ] (17) 1379
6 ρ c = x [ f ρ f + W f ρ ] (18) In terms of fibre volume fraction,v f, the composite density, ρ c, can be written as ρ c = ρ f V f + ρ V f (19) From the assumption of perfect bonding between fibres and matrix, we can write: ε f = ε = ε c (20) Since both fibres and matrix are elastic, the representative longitudinal systems can be calculated as σ f = E f ε f = E f ε c (21) σ = E ε = E ε c (22) Comparing Eq. (21) and Eq. (22) and knowing from material properties that E f E we conclude that the fibre stress σ f > σ. The total tensile load P applied on the composite lamina is shared by fibres and matrix so that P = P f + P (23) Equation (23) can be written as σ c A c = σ f A f + σ A (24) or σ c = σ f A f A c + σ A m A c (25) SinceV f = A f A c and V m = A m A c, the Eq. (25) gives In general, fibre failure strain is lower than the matrix failure strain. Assuming all fibres have the same strength, the tensile rupture of fibres will determine the rupture in the composite. In polymeric matrix composite is E f m >. Thus, even for V f =., fibres carry more than 70% of composite load. Thus, using Eq. (28), the longitudinal tensile strength σ L of a unidirectional continuous fibre can be estimated as σ L = σ f V f + σ V f (30) Where: σ f is fibre tensile strength; σ is matrix stress at fibre failurestrain (ε = ε f ). For effective measurement of the reinforcement of the matrix (σ L σ m, the fibre volume fraction in the composite must be greater than a critical value. This critical volume fraction is calculated by setting σ L = σ m. Thus, from Eq. (30), the value can be calculated as: V f_ciica = [σ σ ][σ f σ ] (31) The fibre weight fraction was computed as 50% using the computer code given in Figure4 agrees with the major requirement of the acceptable range of (±5%) fibre contents to determine elastic constants before using them in the investigation Formulations for coefficients of stiffness and compliance matrices The relationships of composite material properties, relative volume contents, and geometric arrangement of the constituent materials are useful in mechanics of materials models. Engineering constants measured from rule of mixture are used to determine components of lamina the stiffness matrix [] and compliance matrix [] from Eq. (13)(16): σ c = σ f V f + σ V (26) = =σ f V f + σ V f (27) Dividing both sides of the Eq. (27) by ε c and using Eq. (21) & (22), we can write the longitudinal modulus for the composites as E = E f V f + E V f (28) Equation (28) is called the rule of mixture that shows that the composite s longitudinal modulus is intermediate between fibre and matrix moduli. The fraction of load carried by fibres in a unidirectional continuous fibre lamina is P f P = σ fv f [σ f V f + σ V f ] = E f V f [E f V f + E V f ] (29) = = = = = = = = = = (32) The five engineering constants in stiffness/compliance matrices are very useful in the analyses of laminates having multiple laminae in nonprincipal coordinates. Simple relationships of transformation of stress components between coordinate localglobal axes for the wedgedshape differential element can be applied to the equations of static equilibrium of loaded laminates. 1380
7 3.2 Macromechanics methods Formulations for orthotropic lamina The macromechanical stressstrain relations of the lamina can be expressed in terms of an equivalent homogeneous material. However, the properties of the composites are usually anisotropic. In the angleply laminates the principal directions of the orthotropy of each individual ply do not coincide with the generalised coordinate system. Components of the lamina stiffness matrix need to be transformed into a global form with different angles. A unidirectional composite has three mutually orthogonal planes of material property symmetry (i.e., the 12, 23, and 13 planes) and is the orthotropic material. The 123 coordinates are referred as the principal material coordinates since they are associated with reinforcement directions. The lamina is in a twodimensional state of stress (plane stress). The stressstrain relationships can be simplified by letting outofplane shear stresses zero (σ = = = of a thin elastic lamina.the elastic constants influence from inplane deformations have strainstress relationships as: = (σ σ ) = ( σ + σ ) = ( ) (33) Stresses in the xycoordinate system can be transformed for an orthotropic lamina using the localglobal coordinate transformation matrix: σ { σ } = [T] { σ σ } (34) Where:[T] = [ ]; = cos θ a = sin θ The elastic constants ( and )in global coordinates may be determined to relate properties of a lamina in which continuous fibres are aligned at angle θ as shown in Figure5. = c θ = i θ = + ν + + i θ + [ ν ] sin (35) + c θ + [ ν ] sin (36) + ν + ν = E [ ν + ν + cos (37) sin ] (38) ν = ν (39) Figure5. Unidirectional lamina reinforced with rotated fibres. There is no coupling between the shear stresses and normal stress for an orthotropic. The strainstress relations for a lamina in a plane stress form become: = σ σ = σ + σ = σ σ + (40) Coefficients of mutual influence ( and ) for an anglelamina in global coordinates can be determined from the equations: = sin θ [ ν + θ + ν + ] (41) = sin θ [ ν + θ + ν + ] (42) The symmetry presented by the unidirectional lamina makes it socalled orthotropic material. For an especially orthotropic lamina (θ = and ), the stressstrain relations yield: = = σ σ σ = = + σ = = = (43) Using Eq. (32), the relations may be written in local coordinates as: σ { σ } = [ ] { γ } (44) 1381
8 Similarly, for the general orthotropic lamina (θ and ), the complete set of transformation equations for the stresses in the xycoordinate system can be developed using the localglobal coordinate transformation matrix. The generally orthotropic laminate creates fully populated, the reduced transformed stiffness matrix: σ { σ } = [ ] { } (45) Where matrices: [ ] = [T] [][][T][] and Reuter transforms [] = [ ]for strains can be performed in the same manner using tensor strain as engineering shear strain. It is not a tensor quantity and is twice the tensor shear strain ( =. The models given in Eq. (45) are complicated hence semiempirical models have been developed for the design purposes. They can be used over a wide range of elastic properties and fibre volume fractions. The equations are semiempirical in nature since involved parameters in the curve fitting carry physical meaning. The sharp drop in modulus as the angle changes slightly from 0 0 is its limitation since over much of the range of lamina orientation the modulus is very low which requires transverse reinforcement in most composites. The shearcoupling effects are the generation of shear strains by offaxis normal stresses and the generation of normal strains by offaxes shear stresses. The degree of shear coupling is defined by dimensionless shearcoupling ratios or mutual influence coefficients or shearcoupling coefficients. The mutual influence coefficients can be found from:, = γ ε (46) Similarly, when the state of stress is defined as σ, σ = τ =, the ratio, = γ ε (47) Pure shear stresses τ, σ = σ =, the ratio, characterises the normal strain response along the y direction due to a shear stress in the xy plane. The ratio can be found as:, = τ (48) Superposition of loading, stressstrain relations in terms of elastic constants are: { } = s ν η s ν η s η s η s σ { σ } (49) s [ ] The modulus of elasticity and tensile strength of a laminate under a uniaxial load applied in the xdirection at an angle θ to the fibres 1direction may be determined from the transformed reduced stiffness matrix. The moduli: E, E, G, andν in global coordinates can be written as: E = [ m n ν + n m ν + (50) ] E = [ n m ν + m n ν + (51) ] G = [ + ν + + ν + (52) ] ν = E [ m ν n + n ν m + (53) ] ν = E ν E (54) E = G = [ + ν + ν ( ) ] (55) E = G = [ + ν + ν + ( ) ] (56) The Eq. (55) and (56) illustrate an angleply laminate in which the various plies are orientated at ± θ to the plate element axes, in this case the xaxis. The laminates which have an equal member of + θ and θ plies are balanced about their midplane are orthotropic in nature. In the case stresses and strains related by the transformed reduced stiffness matrix: { σ σ σ σ σ σ } = Q Q Q Q ε Q Q Q Q ε Q Q Q ε Q Q γ γ Q [ Q Q Q Q ] { γ } (57) The thirteen constants are related to nine through the following transformation the components of the transformed stiffness matrix defined as follows: 1382
9 = θ + θ + + θ θ Q = Q + Q Q sin cos + Q cos + sin = θ + θ Q = Q cos + Q sin + Q + Q sin cos = θ + θ = Q = Q Q Q sin cos Q Q Q cos sin = cos θ θ sin θ θ = sin θ cos θ = θ + θ = sin θ cos θ = θ + θ = + θ θ + θ + θ (58) Although the transformed  matrix now has the form as that of anisotropic material with nine nonzero coefficients, only four of the coefficients are independent because they can all be expressed in terms of the four independent stiffness of the specially orthotropic material. The lamina engineering constants can also be transformed from principal material axes to the offaxes coordinates. The effects of lamina orientation on stiffness are difficult to assess from inspection stiffness transformation equations. In addition, the eventual incorporation of lamina stiffness over the laminate thickness, and integration of such complicated equations is also difficult. In view of the difficulties, a more convenient form of lamina stiffness transformation equations has been proposed in [12]. By using trigonometric identities to convert from power functions to multiple angle functions and then using additional mathematical manipulations. The invariants are simply linear combinations of the Qij, are invariant to rotations in the plane of the lamina. Thus, the effects of lamina orientation on stiffness are easier to interpret. Invariant formulations of lamina compliance transformations are also orthogonal. From Eq. (29) it appears that there are six constants that govern the stressstrain behaviour of a lamina. However, the equations are linear combinations of the four basic elastic constants, and therefore are not independent. Elements in stiffness matrices can be expresses in terms of five invariant properties of the lamina using trigonometric identities in [21]. The invariants to rotations are simply linear combinations in plane of the lamina. There are four independent invariants, just as there are four independent elastic constants. In all the stiffness expressions (except coupling) consist of one constant term which varies with lamina orientations. Thus, the effects of lamina orientation on stiffness are easier to interpret very useful in computing elements of these matrices. The element of fibrereinforced composite material with its fibre oriented at some arbitrary angle exhibits a shear strain when subjected to a normal stress, and it also exhibits an extensional strain when subjected to a shear stress. The state of stress is defined as whereσ, σ = τ = Formulation for effective constants of laminates The quantities of the elastic constants of every plies in material coordinates were utilised to approximate effective elastic constants for laminated structural element of thickness H made of N plies in global coordinates: = = N N N N = N N ν = N N ν = N N = θ (59) = θ (60) = θ (61) = ν θ (62) = ν θ (63) The effective elastic constants in the xaxis direction E x, in the yaxis direction E y, the effective Poisson s ratios ν xy and ν yx, and the effective shear modulus in the xy plane G xy are computed. As symmetric balanced laminates were considered therefore the following three average laminate stresses were defined [1]: σ = σ = τ = σ z (64) σ z (65) τ z (66) Where: H is the thickness of the laminate. Integration throughthickness in Eq. (64)(66) with was approximated as a summation to obtain the average stresses and related to the force resultants (N, N, andn as: σ = N (67) σ = N (68) τ = N (69) To relate strains to the stresses: { a a } = [ a a a σ ] { σ } (70) The effective elastic constants can be obtained for the laminate using 3 x 3 balanced matrix at RHS in Eq. (70): 1383
10 = = a a = a 66 (71) (72) (73) ν = a a (74) ν = a a (75) The effective Poisson s ratios ν and ν are interdependent and related by the following reciprocal relations: ν Where = ν (76) a = a = a = (77) (78) (79) a = (80) 66 Where: = = [ ] z z, =,, 6; =,, NUMERICAL RESULTS AND DISCUSSION The threedimensional formulations (Equation (45)(51), Equation (56)(60), Equation (59)(63), and Equation (71)(75) were implemented in MATLAB TM V 7.10a code to approximate the elastic constants (see Figure6). Input properties shown in Table2 were assigned to the respective parameters. clear clc %Enter input data e11=input( Enter Ex, e11 ); e22=input( Enter Ex, e22 ); nu12=input( Poisson s ratio, nu12 ); g12=input( Shearmodulus, g12 ); laminate=input( Enter no of plies in laminate, d ); diary Elastic_moduli_ply8.out Q = ReducedStiffness(e11, e22, nu12, g12) Qbar1=Qbar(Q,0);Qbar2=Qbar(Q,90); Qbar3=Qbar(Q,45); Qbar4=Qbar(Q,45); Qbar5=Qbar(Q,45); Qbar6=Qbar(Q,45);Qbar7=Qbar(Q,90);Qbar8=Qbar(Q,0); z1=1.2;z2=0.9;z3=0.6;z4=0.3;z5=0.0;z6=0.3;z7=0.6;z8=0.9;z9=1.2; A=zeros(3,3); A=Amatrix(A,Qbar1,z1,z2);A=Amatrix(A,Qbar2,z2,z3);A=Amatrix(A,Qbar3,z3,z4); A=Amatrix(A,Qbar4,z4,z5);A=Amatrix(A,Qbar5,z5,z6);A=Amatrix(A,Qbar6,z6,z7); A=Amatrix(A,Qbar7,z7,z8);A=Amatrix(A,Qbar8,z8,z9); a = inv(a);y = 1/(H*a(2,2));H=2.4; Exx= Ebarx(A,H) Eyy=Ebary(A,H) Nu12=NUbarxy(A,H) Gxy=Gbarxy(A,H) diary off function y = ReducedStiffness(E1,E2,NU12,G12) %This function returns the reduced stiffness matrix size 3 x 3. NU21 = NU12*E2/E1; y = [E1/(1NU12*NU21) NU12*E2/(1NU12*NU21) 0 ; NU12*E2/(1NU12*NU21) E2/(1NU12*NU21) 0 ; 0 0 G12]; function y = Qbar(Q,theta) %This function returns the transformed reducedstiffness matrix size 3 x 3. m = cos(theta*pi/180);n = sin(theta*pi/180); T = [m*m n*n 2*m*n ; n*n m*m 2*m*n ; m*n m*n m*mn*n]; Tinv = [m*m n*n 2*m*n ; n*n m*m 2*m*n ; m*n m*n m*mn*n]; y = Tinv*Q*T; function y = Amatrix(A,Qbar,z1,z2) %This function returns the matrix after the layer k with stiffness is %assembled. for i = 1 : 3 for j = 1 :
11 A(i,j) = A(i,j) + Qbar(i,j)*(z2z1); end end y = A; function y = Ebarx(A,H) %This function returns the average laminate modulusin the xdirection. a = inv(a);y = 1/(H*a(1,1)); function y = NUbarxy(A,H) %This function returns the average laminate Poisson s ratio NUxy. a = inv(a);y = a(1,2)/a(1,1); function y = Ebary(A,H) %This function returns the average laminate modulus a = inv(a); y = 1/(H*a(2,2)); function y = Gbarxy(A,H) %This function returns the average laminate shear modulus. a = inv(a);y = 1/(H*a(3,3)); Figure6. MATLAB TM code to compute engineering constants. The data obtained from the simulations were plotted against fibres rotated plies in the laminates. The plots highlight the relation between elastic constants at various angles. The code for plots of effective values of four elastic constants as a function of orientation angle in the range: θ π at the difference of 10 degrees is shown Figure7. clear clc %Enter input data e11=input( Enter Ex, e11 ); e22=input( Enter Ex, e22 ); nu12=input( Poisson s ratio, nu12 ); g12=input( Shearmodulus, g12 ); laminate=input( Enter no of plies in laminate, d ); diary Elastic_Constants.out fprintf('====== Angle and Elastic constants ======\n'); fprintf(' \n\n') fprintf('angle \texx v12 Eyy Gxy \n'); fprintf('===== \t======= \t======= \t======= ======== \n'); i=0; for ii = 0:10:90 i=i+1; ex1(i) = Ex(e11,e22, nu12, g12, ii); nuxy(i) = NUxy(e11,e22, nu12, g12, ii); ey2(i) = Ey(e11,e22, nu12, g12, ii); nuyx(i) = NUyx(e11,e22, nu12, g12, ii); gxy(i) = Gxy(e11,e22, nu12, g12, ii); fprintf('%2d \t\t%5.2f\t\t%5.2f\t\t%5.2f\t\t%5.2f\n',ii, ex1(i),nuxy(i),ey2(i), gxy(i)) disp('elastic constant') disp(ex1(i)) plot(ii,ex1(i)); xlabel('angle, \theta (degree)'); ylabel('e_{xx}(gpa)'); title('elasitic modulus E_{xx} v Rotation','FontSize',14) plot(ii,nuxy(i)); xlabel('angle, \theta (degree)'); ylabel('\nu_{xy}'); title('elasitic modulus \nu_{xy} v Rotation','FontSize',14); plot(ii,ey2(i)); xlabel('angle, \theta (degree)'); ylabel('e_{yy}(gpa)'); title('elasitic modulus E_{yy} v Rotation','FontSize',14'); plot(ii,gxy(i)); 1385
12 xlabel('angle, \theta (degree)'); ylabel('g_{xy}(gpa)'); title('shear modulus G_{xy} v Rotation','FontSize',14); diary off Figure7. MATLAB TM code to plot engineering constants v rotations. Plots of the effective engineering constants of an8ply laminate as a function of angle orientations in the range: θ π at the difference of 10 degrees are selected for discussion. The plot in Figure8 illustrates quantities of Young s modulus in parallel to fibre (xaxis) directions. Variation of the curve shows maximum value around 230GPa as expected when fibres were aligned at zerodirections. It shows severe drop as angle increases from 0 0 and this trend continues until angle reaches 90 0 where value of the modulus drops to around 23GPa. Changes in quantities of Young s moduli with respect to rotations indicate that simulation obtain values are realistic. Figure9. Poisson s ratios v ply orientation. Figure10 illustrates quantities of Young s modulus in perpendicular to fibre (yaxis) directions. Variation of the curve shows minimum value around 23GPa as expected when fibres were aligned at It shows increasing trend as angle increases from 0 0 and this trend continues until angle reaches 90 0 where value of the modulus reaches to around 230GPa. Changes in quantities of Poisson s ratio with respect to rotations confirm that simulation obtain values are realistic. Figure8. Yong s moduli in fibre direction v ply orientation. Figure9 illustrates quantities of Poisson s ratios. Variation of the curve shows gradual drop of the values from 0.2 maximum when fibres are aligned at 0 0 rotations and minimum around 0.02 fibres were aligned at The curve shows decreasing trend as angle increases from 0 0 and this trend continues until angle reaches Changes in quantities of Young s moduli with respect to rotations support the arguments that simulations obtain values are realistic. Figure10. Young s moduli in perpendicular to fibres v ply orientation. Figure11 illustrates quantities of shear moduli. Variation of the curve follows parabolic path. Maximum values of 88GPa at fibre directions 0 0 can be seen which gradually to minimum around 20GPa at fibre direction 45 0 and then reverse trend begins up to 90 0 where it again reaches to 88GPa. Such types of variations were expected and that confirmed that the predicted quantities are realistic and genuine. Changes in quantities of shearmoduli with respect to rotations also confirm that simulation obtain values are realistic. 1386
13 5. VALIDATION OF SIMULATION OBTAINED ENGINEERING CONSTANTS Figure11. Shear moduliv ply orientation. Since elastic constants are interdependent hence elastic constants were computed for all the laminates. For the especially orthotropic and transversally isotropic the constants are G 12, G 13 ; E 2 = E 3 ; 21 = 31, and 23 = 32. In addition, the relationship among the isotropic engineering constants Eq. (61) is valid associated with the 23 plane, so that G =. Effective values for Young s moduli +ν for all the laminates are shown in Table4. Table4. Simulation obtained Young s moduli. Laminate Layup Effective Young s moduli No of ply Code GPa 8Ply [0/90/45/45] S Ply [0/90/45/45] 2S Ply [0/90/45/45] 3S Rule of mixture The elastic properties were calculated utilising the respective volume fractions in Eqns. (25)(28) for 8, 16, and 24Ply laminates. Identical averaged Young s moduli E 1 and transverse E 2 were obtained due to quasiisotropic configuration of the laminates with fibre volume fraction for all the laminates with three different thicknesses. Quantities of the Poisson s ratios and inplane shearmoduli also computed and good agreement of the intrasimulated values for every laminate was found. Since engineering constants are interdependent Young s moduli suffice the requirements. Hence Young s moduli calculated from the volume fraction equations are given in Table5. Table5. Young s moduli computed using Rule of Mixture. Laminate Young s modulus Layup No of ply GPa Code 8Ply 58.5 [0/90/45/45] S 16Ply 58.6 [0/90/45/45] 2S 24Ply 58.8 [0/90/45/45] 3S 5.2 Hart smith rule The Hart Smith Rule used to calculate the elastic modulus of the laminates. The determined elastic constant for the quasiisotropic configuration is calculated and shown in Table6. Table6. Young s modulus determined from Hart Smith rule. Supplied elastic modulus 230 GPa comes down to GPa for 54% contents. Sequence: [45/0/45/90] Hart Smith Rule Angle (degree) Multiple Modulus Modulus of the 4ply quasiisotropic laminate ( )/4 Equivalent to the unidirectional GPa 5.3 Tensile test experiment Three laminates from each of the coupon types were prepared in Ishapes in line with the testing standard for tensile tests (ASTM: D3039). Average span and width of each laminate was 120 mm and 20 mm, respectively. Thicknesses (t = 2.4, 4.8, and 7.2 mm) from each of the layup of 8, 16, and 24Ply varied due to number of plies within the stacks. Load transfer tabs were adhesively bonded to the ends of the laminates in order that the load may be transferred from the grips of the tensile testing machine to the laminate without damaging the laminate. Laminates were gripped at both ends. Approximate dimensions and relevant spans to depth ratios are shown in Figure
14 Figure12. Schematic of beam laminates with crosssection. The effective beam length (L) used for all calculations was length (120 mm)  both the grips (30 mm) = 90 mm. Average geometrical dimensions can be seen in Table7 below. Table7. Beams layup configuration and geometrical dimensions. Configuration Grip: d Grip: c Thickness: t Effective length: L Mm [45/90/0/45] s [45/90/0/45] 2s [45/90/0/45] 3s Photographs of the laminates selected for the tests are shown in Figure13(a). The laminates were inserted within in the fixture holders of the machine by metal grips as shown in Figure13(b) and loaded axially at a rate of 1mm/min. The applied tensile load produced tensile stresses through the holding grips that results elongation of the laminate in loading direction. The applied tensile loading and corresponding voltage output values were recorded by the software installed on the data acquisition system at specified load increments so that the curve is plotted for each and every test data. Measurements for the strains were correlated from the recorded voltage ranges and scaled by the gain from the formula  given = e. Where: is output v K voltage (needs to be divided by gain of 341), v is bridge excitation voltage (its value is: 5v), K is the gainfactor (equal to: 2.13). Behaviour of the laminate was observed while load was being applied through variation in output voltage quantities during the tests of every laminate. Most of the results have shown consistency and linearity for the longitudinal strain response through system builtin display screen. A slight nonlinearity in the strain response was observed due to the influence of the matrix properties. Measurements of the strains and loads were used to determine the elastic modulus. Stresses were calculated from the applied loads on the respective areas. The recorded strains and calculated stresses were used to determine the Young s modulus as shown in Table8. Mean moduli were calculated for the every laminate. Independent tests for every laminate were carried out for each of the laminates. Figure13. Photographs of: a) laminate and b) INSTRON TM 5585H machine. 1388
15 Table8. Tensile test results. Laminate Elastic Voltage Microstrain area mm 2 Load KN modulus Crosssectional Stress Thickness (range) Test GPa mm GPa T T T T T T Flexural test experiment There is a wide variety of test methods available for flexure testing described (ASTM: D7264) addressing the particular needs of heterogeneous nonisotropic materials. In general, flexure test type tests are applicable to quality control and material selection where comparative rather than absolute values are required. Flexural properties of the laminates were determined using the standard three point bending test method. For flexure test, there is no involvement of endtabs or changes in the laminate shape. Tests can be conducted on simply supported beams of constant crosssectional area. A schematic of simply supported beam at close to ends flat rectangular laminate is shown in Figure14(a). The laminate is centrally loaded representing threepoint bending test. Dimensions of the three laminates with crosssectional areas having constant width but different thicknesses are shown in Figure14(b). Figure14. Schematics: a) laminate bending and b) crosssectional area. Approximate dimensions and relevant simple support of span to depth ratios provides base to formulation the calculation of Young s modulus from the loaddisplacement relation given in Table9. Table9. Formulation used to calculate young s modulus. Bending moment = Moment of area = w Max bending stress Load Young s modulus σ a = = w = σw = The machine shown in Figure13 is used with changed testing chamber. Two laminates from the three types of laminates were selected and atypical one is shown in Figure15(a) with test chamber in (b). The laminates were placed in the fixture and gradually loaded. The laminates were held in place in the machine in flexural test chamber and gradually loaded. During flexural tests all of the laminates experienced deflection under increased loading. The deflection typically occurred at the middle of the laminates, which was in contact with the machine head, therefore considered to be a loaded edge. The loading produces the maximum bending moment and maximum stress under the loading nose. The vertical load could deflect (bend) the laminate and even fracture the outer fibres of the laminate under excessive loading. 1389
16 Figure15. a) Test laminate b) test chamber of INSTRON TM 5585H. The strain values and the other data were recorded by software installed on the data acquisition system at specified load increments so that the curve is plotted for each laminate. In the beginning of the bending test the loaddeflection curves show slightly erratic behaviour, but along the course of the curves there is a definable linear portion. Independent tests for every laminate were carried out and mean moduli were calculated for the every laminate. Measurements of the strain values, deflections and loads were used to determine the Young s modulus. As shown in Table10 below the recorded voltage range was scaled by gain factor and strains values were calculated. Stresses were calculated from the recorded applied load divided by the corresponding crosssectional area. Young s moduli were then calculated using the strain and stress values and have been shown in column 8 of Table10. Table10. Flexural test results. Elastic modulus Test Laminate Bridge factor Microstrain Load N Stress GPa GPa B Ply B B Ply B B Ply B Overall comparison of approximated elastic moduli Selected young s moduli for all the 8, 16, and 24Ply laminates obtained from simulation, rule of mixture, Hart Smith, tensile, and flexural testing methodologies are compared in Table11. Good agreement of the predicted values of Young s moduli for every laminate was found. The comparisons confirmed that results of the mechanical properties (physical plus elastic stiffness) delivered from the MATLAB TM programs are reliable. Table11. Comparison of Young s moduli from different methods. Methodologies applied Laminate Simulation Rule of Hart mixture Smith Tensile Flexural Young s modulus GPa 8Ply Ply Ply CONCLUSIONS In this investigation, engineering properties of quasiisotropic 8, 16, and 24Ply carbon fibrereinforced laminated composite panels were determined applying simulation methodology based on micromacro mechanics of the laminates. Physical properties were determined and ignition loss tests were conducted to evaluate volume fractions quantities from the rule of mixture. The rule of mixture and inverse rule of mixture were utilised to approximate engineering constants. Then twodimensional stressstrain relation and micromacro mechanics methods were applied to formulate lamina, angle lamina, and threedimensional laminate elements. Computer codes were developed to determine range of the engineering constants. Selected data obtained from the simulations were verified with tensile and flexural physical testing. Based on comparison of the results the following conclusions can be extracted: 1390
17 Micromacro mechanics of a lamina were utilised to approximate effective elastic constants for threedimensional laminates. Simulation produced results were validated against the values obtained by volume fractions and Hart Smith rules, tensile, and flexural testing and were found to be within acceptable range with (±10%) deviations. Elastic constants determined from MATLAB TM simulations were also compared to the intrasimulation values as a function of fibre rotations and were found to be in good agreement. Based on comparisons of the results it is proposed that threedimensional (full range) of effective elastic constants can be efficiently determined from information of the volume fraction, twodimensional micromechanics laws, and computer simulations with reduced physical testing. REFERENCES [1] Morgan P Carbon Fibres and their composites. Taylor & Francis, Boca Raton, USA. [2] Yang B, Kozey V, Adanur S, Kumar S Bending, compression, and shear behaviour of woven glass fibre epoxy composites. Composites: Part B. 31: [3] Hussain SA, Reddy SB and V, and Reddy VN Prediction of elastic properties of FRP composite lamina for longitudinal loading. Asian Research Publishing Network. 3(6): [4] Gao XL, Li K, and Mall S A mechanicsofmaterials model for predicting Young s modulus of damaged woven fabric composites, involving three damage modes, Int J Solids Struct. 40: [5] John EL, XiaowenY, Mark IJ Characterisation of voids in fibre reinforced composite materials. NDT&E International. 46: [6] Keshavamurthy YC, Nanjundaradhya NV, Ramesh SS, Kulkarni RS Investigation of tensile properties of fibre reinforced angle ply laminated composites. Int. J Emerg Technol Adv Eng. 2(4): [7] Emilia S, Nicolai B and Paul B Mechanical characteristics of composite materials obtained by different technologies. Academic J Manufactur Eng. 9(3): [8] Altaf HS, PandurangaduV, Amba PRG Prediction of elastic constants of carbon T300/ epoxy composite using soft computing. Int J Inn Research in Sci Eng Technol. 2(7): [9] Bradley LR, Bowen CR, McEnaney B, Johnson LR Shear properties of a carbon/carbon composite with nonwoven felt and continuous fibre reinforcement layers. Carbon. 45: [10] Mujika F On the difference between flexural moduli obtained by threepoint and fourpoint bending tests. Poly Testing. 25: [11] Satish KG, Siddeswarappa B, Mohamed KK Characterization of inplane mechanical properties of laminated hybrid composites. J Miner Mater Character Eng. 9(2): [12] Irina P, Cristina M, Constant I The determination of Young modulus for cfrp using three point bending tests at different span lengths. Scientific BulletinUniversity Politehnica of Bucharest. 75: [13] Konrad Gliesche, Tamara Hubner, Holger Orawetz Investigations of inplane shear properties of ±45 0 carbon/epoxy composites using tensile testing and optical deformation analysis. Compos Sci Technol. 65: [14] Bradley LR Mechanical testing and modelling of carboncarbon composites for aircraft disc brakes. PhD thesis, University of Bath, UK. [15] Barbero EJ Introduction to composite materials design, (Second Edition), CRC Press Taylor & Francis Group. [16] D. Bhagwan, Agarwal and Lawrence J Broutman, Analysis and Performance of Fibre Composites. John Wiley and Sons Inc, Unites States. [17] Romano F., Fiori J., Mercurio U. May Structural Design and Test Capability of a CFRP Aileron. Composite Structures. 88(3): [18] Liyong Tong, Adrian P. Mouritz and Michael K Bannister '3D Fibre Reinforced Polymer Composites' Book, Elsevier Science Ltd. All Rights Reserved. 1391
18 [19] Prashanth Banakar1, H.K. Shivananda2 and H.B. Niranjan Influence of Fibre Orientation and Thickness on Tensile Properties of Laminated Polymer Composites. Int. J. Pure Appl. Sci. Technol. 9(1): [20] F. Mujika On the difference between flexural moduli obtained by threepoint and fourpointbending tests, Polymer Testing. 25: [21] F. Gibson Principles of composite materials mechanics. Taylor & Francis Group, CRC Press Boca Raton. pp
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More informationElastic parameters prediction under dynamic loading based on the. unit cell of composites considering end constraint effect
Elastic parameters prediction under dynamic loading based on the unit cell of composites considering end constraint effect Wang Meng 1,, Fei Qingguo 1,, Zhang Peiwei 1, (1. Institute of Aerospace Machinery
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More informationA FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE
A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering,
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE MATERIAL
5 th International Conference Advanced Composite Materials Engineering COMAT 2014 1617 October 2014, Braşov, Romania ASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More information*Corresponding author: Keywords: Finiteelement analysis; Multiscale modelling; Onset theory; Dilatational strain invariant.
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MICROMECHANICAL MODELLING OF TEST SPECIMENS FOR ONSET OF DILATATIONAL DAMAGE OF POLYMER MATRIX IN COMPOSITE MATERIALS T. D. Tran 1, D. Kelly 1*, G.
More informationDetermination of the Shear Buckling Load of a Large Polymer Composite ISection Using Strain and Displacement Sensors
Sensors 2012, 12, 1602416036; doi:10.3390/s121216024 Article OPEN ACCESS sensors ISSN 14248220 www.mdpi.com/journal/sensors Determination of the Shear Buckling Load of a Large Polymer Composite ISection
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationThe Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints
, June 30  July 2, 2010, London, U.K. The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints O. Aluko, and Q. Mazumder Abstract An analytical model was developed
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 15 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationA synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks
Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More information2D damping predictions of fiber composite plates: Layup effects
Available online at www.sciencedirect.com Composites Science and Technology 68 (2008) 727 733 COMPOSITES SCIENCE AND TECHNOLOGY www.elsevier.com/locate/compscitech 2D damping predictions of fiber composite
More informationCellular solid structures with unbounded thermal expansion. Roderic Lakes. Journal of Materials Science Letters, 15, (1996).
1 Cellular solid structures with unbounded thermal expansion Roderic Lakes Journal of Materials Science Letters, 15, 475477 (1996). Abstract Material microstructures are presented which can exhibit coefficients
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationTESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS
TESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS I. M. Daniel, J. L. Abot, and K. A. Wang Walter P. Murphy Professor, Departments of Civil and Mechanical Engineering, Robert R. McCormick School of Engineering
More informationNigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37
Nigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37 APPLICATION OF THE REISSNERS PLATE THEORY IN THE DELAMINATION ANALYSIS OF A THREEDIMENSIONAL, TIME DEPENDENT, NONLINEAR, UNIDIRECTIONAL
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationA SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST
A SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST P. Robinson The Composites Centre, Department of Aeronautics, Imperial College London South Kensington, London, SW7 2AZ, UK p.robinson@imperial.ac.uk
More informationUSING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE
Volume II: Fatigue, Fracture and Ceramic Matrix Composites USING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE A. D. Resnyansky and
More informationPresented By: EAS 6939 Aerospace Structural Composites
A Beam Theory for Laminated Composites and Application to Torsion Problems Dr. BhavaniV. Sankar Presented By: Sameer Luthra EAS 6939 Aerospace Structural Composites 1 Introduction Composite beams have
More informationCOMPUTER AIDED DESIGN IN CASE OF THE LAMINATED COMPOSITE MATERIALS
6 th International Conference Computational Mechanics and Virtual Engineering COMEC 15 1516 October 15, Braşov, Romania COMPUER AIDED DESIGN IN CASE OF HE LAMINAED COMPOSIE MAERIALS Camelia Cerbu ransilvania
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationLaboratory 4 Bending Test of Materials
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
More informationFRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT  Institut Supérieur de l Automobile et des Transports, LRMA  Laboratoire de
More information6. Bending CHAPTER OBJECTIVES
CHAPTER OBJECTIVES Determine stress in members caused by bending Discuss how to establish shear and moment diagrams for a beam or shaft Determine largest shear and moment in a member, and specify where
More informationComposite Laminate Modeling
omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationMicromeso draping modelling of noncrimp fabrics
Micromeso draping modelling of noncrimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Noncrimp fabrics (NCFs) are
More informationIraq Ref. & Air. Cond. Dept/ Technical College / Kirkuk
International Journal of Scientific & Engineering Research, Volume 6, Issue 4, April015 1678 Study the Increasing of the Cantilever Plate Stiffness by Using s Jawdat Ali Yakoob Iesam Jondi Hasan Ass.
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationInternational Journal of Advanced Engineering Technology EISSN
Research Article INTEGRATED FORCE METHOD FOR FIBER REINFORCED COMPOSITE PLATE BENDING PROBLEMS Doiphode G. S., Patodi S. C.* Address for Correspondence Assistant Professor, Applied Mechanics Department,
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 4 MICRO MECHANICS. E E v E E E E E v E E + + = m f f. f f
MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown
More informationModule 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory. Introduction: The Lecture Contains: Laminate Theory with Thermal Effects
Module 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory Introduction: In this lecture we are going to develop the laminate theory with thermal and hygral effects. Then we will develop the
More informationAPPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN
28 TH INTERNATIONAL CONGRESS OF THE AERONAUTICAL SCIENCES APPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN Tuyen Tran*, Dan Simkins**, Shen Hin Lim*,
More informationStacking sequences for Extensionally Isotropic, Fully Isotropic and QuasiHomogeneous Orthotropic Laminates.
49th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials 710 April 2008, Schaumburg, IL AIAA 20081940 Stacking sequences for Extensionally Isotropic, Fully Isotropic and QuasiHomogeneous
More information7.4 The Elementary Beam Theory
7.4 The Elementary Beam Theory In this section, problems involving long and slender beams are addressed. s with pressure vessels, the geometry of the beam, and the specific type of loading which will be
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationEffects of geometry and properties of fibre and matrix on overall. composite parameters
Int. Journal of Applied Sciences and ngineering Research, ol. 3, Issue 4, 2014 www.ijaser.com 2014 by the authors Licensee IJASR Under Creative Commons License 3.0 editorial@ijaser.com Research article
More informationFEM Modeling of a 3D Printed Carbon Fiber Pylon
FEM Modeling of a 3D Printed Carbon Fiber Pylon I. López G.*, B. Chiné, and J.L. León S. Costa Rica Institute of Technology, School of Materials Science and Engineering, Cartago, Costa Rica *Corresponding
More informationEFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES
EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES OF WOOD OR PLYWOOD CONSIDERED AS ORTHOTROPIC MATERIALS Information Revied and Reaffirmed March 1956 No. 1510 EFFECT OF ELLIPTIC
More informationAE3610 Experiments in Fluid and Solid Mechanics TRANSIENT MEASUREMENTS OF HOOP STRESSES FOR A THINWALL PRESSURE VESSEL
Objective AE3610 Experiments in Fluid and Solid Mechanics TRANSIENT MEASUREMENTS OF OOP STRESSES FOR A TINWA PRESSURE VESSE This experiment will allow you to investigate hoop and axial stress/strain relations
More information4.MECHANICAL PROPERTIES OF MATERIALS
4.MECHANICAL PROPERTIES OF MATERIALS The diagram representing the relation between stress and strain in a given material is an important characteristic of the material. To obtain the stressstrain diagram
More informationBasic Energy Principles in Stiffness Analysis
Basic Energy Principles in Stiffness Analysis StressStrain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationCORRELATING OFFAXIS TENSION TESTS TO SHEAR MODULUS OF WOODBASED PANELS
CORRELATING OFFAXIS TENSION TESTS TO SHEAR MODULUS OF WOODBASED PANELS By Edmond P. Saliklis 1 and Robert H. Falk ABSTRACT: The weakness of existing relationships correlating offaxis modulus of elasticity
More informationApplication of fracture mechanicsbased methodologies for failure predictions in composite structures
Application of fracture mechanicsbased methodologies for failure predictions in composite structures Zoltan Mikulik a, B. Gangadhara Prusty a, Rodney S. Thomson b, Donald W. Kelly a,* a School of Mechanical
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationPlane Strain Test for Metal Sheet Characterization
Plane Strain Test for Metal Sheet Characterization Paulo Flores 1, Felix Bonnet 2 and AnneMarie Habraken 3 1 DIM, University of Concepción, Edmundo Larenas 270, Concepción, Chile 2 ENS  Cachan, Avenue
More informationEVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS T. Kurashiki 1 *, Y. Matsushima 1, Y. Nakayasu
More informationMechanics of Irregular Honeycomb Structures
Mechanics of Irregular Honeycomb Structures S. Adhikari 1, T. Mukhopadhyay 1 Chair of Aerospace Engineering, College of Engineering, Swansea University, Singleton Park, Swansea SA2 8PP, UK Sixth International
More informationAgnieszka Bondyra, Pawe Gotowicki
Journal of KONES Powertrain and Transport, Vol. 17, No. 1 21 INFLUENCE OF A CROSSHEAD RATE AND A NUMBER OF STRESS CYCLES ON MEASUREMENT RESULTS IN THE INPLANE SHEAR TEST FOR A CROSSPLY VINYLESTERCARBON
More informationPLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS PLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES P. Tesinova Technical University of Liberec, Faculty of Textile
More informationPrediction of Compressive Strength of Fibrous Composites Using Two Different Approaches
Jordan Journal of Civil Engineering, Volume 8, No. 2, 214 Prediction of Compressive Strength of Fibrous Composites Using Two Different Approaches Yousef S. Al Rjoub 1) * and Karim S. Numayr 2) 1) Civil
More informationCHAPTER 6 BENDING Part 1
Ishik University / Sulaimani Civil Engineering Department Mechanics of Materials CE 211 CHAPTER 6 BENDING Part 11 CHAPTER 6 Bending Outlines of this chapter: 6.1. Chapter Objectives 6.2. Shear and
More informationAim of the study Experimental determination of mechanical parameters Local buckling (wrinkling) Failure maps Optimization of sandwich panels
METNET Workshop October 1112, 2009, Poznań, Poland Experimental and numerical analysis of sandwich metal panels Zbigniew Pozorski, Monika ChudaKowalska, Robert Studziński, Andrzej Garstecki Poznan University
More informationFinite Difference Dynamic Analysis of Railway Bridges Supported by Pasternak Foundation under Uniform Partially Distributed Moving Railway Vehicle
, October 2123, 2015, San Francisco, USA Finite Difference Dynamic Analysis of Railway Bridges Supported by Pasternak Foundation under Uniform Partially Distributed Moving Railway Vehicle M. C. Agarana
More information2. Mechanics of Materials: Strain. 3. Hookes's Law
Mechanics of Materials Course: WB3413, Dredging Processes 1 Fundamental Theory Required for Sand, Clay and Rock Cutting 1. Mechanics of Materials: Stress 1. Introduction 2. Plane Stress and Coordinate
More informationDESIGN OF COMPOSITE LAMINATED STRUCTURES BY POLAR METHOD AND TOPOLOGY OPTIMISATION
DESIGN OF COMPOSIE LAMINAED SUCUES BY POLA MEOD AND OPOLOGY OPIMISAION A. Jibawy,,3, C. Julien,,3, B. Desmorat,,4, (*), A. Vincenti UPMC Univ Paris 6, UM 79, Institut Jean Le ond d Alembert B.P. 6 4, place
More informationFASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES G. Catalanotti 1*, P.P. Camanho 1, P. Ghys 2, A.T. Marques 1 1 DEMec, Faculdade de Engenharia, Universidade
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationInfluence of residual stresses in the structural behavior of. tubular columns and arches. Nuno Rocha Cima Gomes
October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:
More informationDETERMINATION OF YOUNG S MODULUS FOR CFRP USING THE THREE POINT BENDING TEST
Proceedings in Manufacturing Systems, Volume 6, Issue 4, 2011 ISSN 20679238 DETERMINATION OF YOUNG S MODULUS FOR CFRP USING THE THREE POINT BENDING TEST Irina PETRESCU 1,*, Cristina MOHORA 2, Constantin
More informationPoisson s ratio as a sensitive indicator of (fatigue) damage in fibrereinforced plastics
10.1111/j.14602695.2007.01095.x Poisson s ratio as a sensitive indicator of (fatigue) damage in fibrereinforced plastics W. VAN PAEPEGEM, I. DE BAERE, E. LAMKANFI and J. DEGRIECK Ghent University, Department
More informationSemiMembrane and Effective Length Theory of Hybrid Anisotropic Materials
International Journal of Composite Materials 2017, 7(3): 103114 DOI: 10.5923/j.cmaterials.20170703.03 SemiMembrane and Effective Length Theory of Hybrid Anisotropic Materials S. W. Chung 1,*, G. S. Ju
More informationFinite Element Analysis Prof. Dr. B. N. Rao Department of Civil Engineering Indian Institute of Technology, Madras. Module  01 Lecture  11
Finite Element Analysis Prof. Dr. B. N. Rao Department of Civil Engineering Indian Institute of Technology, Madras Module  01 Lecture  11 Last class, what we did is, we looked at a method called superposition
More informationUnderstand basic stressstrain response of engineering materials.
Module 3 Constitutive quations Learning Objectives Understand basic stressstrain response of engineering materials. Quantify the linear elastic stressstrain response in terms of tensorial quantities
More informationModeling of the Bending Stiffness of a Bimaterial Beam by the Approximation of OneDimensional of Laminated Theory
. FloresDomínguez Int. Journal of Engineering Research and Applications RESEARCH ARTICLE OPEN ACCESS odeling of the Bending Stiffness of a Bimaterial Beam by the Approimation of OneDimensional of Laminated
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 3
MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationGeneric Strategies to Implement Material Grading in Finite Element Methods for Isotropic and Anisotropic Materials
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Engineering Mechanics Dissertations & Theses Mechanical & Materials Engineering, Department of Winter 1292011 Generic
More informationDelamination in fractured laminated glass
Delamination in fractured laminated glass Caroline BUTCHART*, Mauro OVEREND a * Department of Engineering, University of Cambridge Trumpington Street, Cambridge, CB2 1PZ, UK cvb25@cam.ac.uk a Department
More informationA CRITERION OF TENSILE FAILURE FOR HYPERELASTIC MATERIALS AND ITS APPLICATION TO VISCOELASTICVISCOPLASTIC MATERIALS
MTS ADHESIVES PROGRAMME 19961999 PERFORMANCE OF ADHESIVE JOINTS Project: PAJ1; Failure Criteria and their Application to ViscoElastic/ViscoPlastic Materials Report 2 A CRITERION OF TENSILE FAILURE FOR
More informationCentrifuge Shaking Table Tests and FEM Analyses of RC Pile Foundation and Underground Structure
Centrifuge Shaking Table s and FEM Analyses of RC Pile Foundation and Underground Structure Kenji Yonezawa Obayashi Corporation, Tokyo, Japan. Takuya Anabuki Obayashi Corporation, Tokyo, Japan. Shunichi
More informationDELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS
DELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS L Iannucci 1, M S I Shaik Dawood 1,2,3, E Greenhalgh 1 and A K Ariffin 3 1 Aeronautics Department, Imperial College London, South Kensington
More informationA simple planestrain solution for functionally graded multilayered isotropic cylinders
Structural Engineering and Mechanics, Vol. 24, o. 6 (2006) 000000 1 A simple planestrain solution for functionally graded multilayered isotropic cylinders E. Pan Department of Civil Engineering, The
More informationOverview of Hygrothermally Stable Laminates with Improved Extensiontwist Coupling
Overview of Hygrothermally Stable Laminates with Improved Extensiontwist Coupling R. Haynes epartment of erospace Engineering, Georgia Institute of Technology 27 Ferst rive W, tlanta, G 33325, US robert.haynes@gatech.edu
More information